AbstractThe electrical conductivity of Namontmorillonite suspensions in various salt and clay con centrations was measured. The weight conductance of theĀ ...
Clays and Clay Minerals, Vol. 23, pp. 205 210. Pergamon Press 1975. Printed in Great Britain
ELECTRICAL CONDUCTIVITY OF N a  M O N T M O R I L L O N I T E SUSPENSION S* I. S H A I N B E R G
and RACHEL LEVY
Institute of Soils and Water. A.R.O., Volcani Center, Bet Dagan, Israel (Received 9 April 1974) AbstractThe electrical conductivity of Namontmorillonite suspensions in various salt and clay concentrations was measured. The weight conductance of the clay suspension was found to decrease with increase in clay concentration between 0 and approximately 0.5 g clay/100 ml, then rose to a plateau at 610 g clay/100 ml. The weight conductance of the clay suspensions also increased with an increase in the salt solution concentration. If the model of two resistors in parallel is used in interpreting the experimental data, these changes can be attributed to an increase in the mobility of the adsorbed Na ions. It is proposed that the two resistors in series model is more realistic in describing the conductivity of the suspensions. This model predicts the observed weight conductance changes of the suspensions, while the mobility of the adsorbed ions remains constant. A constant mobility of the adsorbed Na ions in claywater systems of low to medium salt and clay concentrations also is predicted by the diffuse double layer. INTRODUCTION
Ionic migration in clay systems is involved in such processes as nutrient uptake by plants, soil formation, salination and reclamation of saline soils and many others. One of the convenient ways of determining the ionic mobility is by measuring the electrical conductivity of the claywater system. Despite its importance, and despite the fact that the electrical conductivity of Namontmorillonite suspensions has been studied by many workers (Van Olphen, 1957; Van Olphen and Waxman, 1958; Low, 1958; Cremers and Laudelout, 1965; Gast, 1966; Davey and Low, 1968; Jorgensen and Low, 1970), there is still much to be learned. All workers found that there is a rapid drop in the weight conductance of Namontmorillonite suspensions at a clay concentration range between 0 and 0'5 g/100 ml, but no satisfactory explanation was offered. Van Olphen and Waxman (1958) suggested that this drop may be due to an increase in electrophoretic and relaxation retardation brought about by compression of the electrical double layer as the particles come closer together. This explanation can hardly be applied to 0.5 g clay in 100 ml solution of 103NNaC1, where the thickness of the diffuse double layer (I/K) is about 100A and the average half distance between the clay platelets is 2600A. Jorgensen and Low (1970) attributed the drop in weight conductance mainly to a decrease in the fraction of exchangeable Na + outside the plane of shear. They did not give any explanation why the fraction of exchangeable Na + outside the plane of shear will drop at this very dilute clay concentration. Between about 0'5 and 6"0 g clay/100ml there was an increase in weight conductance (Van Olphen, 1957; Van Olphen and Waxman, 1958; Jorgensen and Low, 1970). Van Olpben and Waxman (1958) suggested that at a clay concentration above 0.5 g/100 ml,
the particles start to interact. At this point immobilization of the particles and bridging between the electrodes gradually eliminate the retardation effects and surface conductance takes place, Jorgensen and Low (1970) ascribed this increment in weight conductance to an increase in the fraction of exchangeable Na + outside the plane of shear. Again, there was no explanation why the fraction of Na + outside the plane of shear increased with further increase of the clay concentration, Both explanations failed to describe quantitatively the increase in weight conductance with clay concentration at the medium clay concentration range. There is an apparent contradiction between the theoretical prediction and the experimental observation on the effect of electrolyte concentration on the conductivity of clays also. The theoretical prediction was discussed at length by Van Olphen and Waxman (1958). They concluded that since the charge of the clay double layer is determined mainly by imperfections within the clay lattice, the addition of electrolyte does not change the total double layer charge. The counter ion atmosphere is compressed on electrolyte addition and there is a shift of courger ions to the space between the slipping plane and surface; thus, a decrease of the specific surface conductance should take place. In contrast to this prediction, Waxman and Smits (1968), reviewing the abundance of experimental data for the electrical conductivity of shaly formations, observed that in the dilute range of salt concentration there is a sharp increase in conductance with increasing concentration of electrolyte. They attributed this effect to an increase in the mobility of exchangeable ions. Similar measurements on exchange resin (Sauer et al., 1955) and clays (Gast, 1966; Gast and Spalding, 1966; Letey and Klute, 1960) indicated also that addition of a free electrolyte caused a greater increase in electrical conductivity and diffusion rates than that predicted by the increase in the solution conductivity. The purpose of this study was to find the cause of these contradictions. Electrical conductivity of N a 
* Contribution from the Institute of Soils and Water, A.R.O., Volcani Center, Bet Dagan, Israel. 1974 Series, No. 123E. Part of the work was done at the Agronomy Department, Purdue University, West Lafayette, Indiana, U.S.A. 205
206
I. SHAINBERG and RACHEL LEVY
montmorillonite suspensions as functions of clay and electrolyte concentration was measured. The data were analyzed by two different models. THEORY
The electrical conductance of a clay gel can be considered to be due to the contribution of the colloidal particles and the ions present in solution, In a more schematic way the electrical conductivity can be split up into the contribution of the clay particles and their counter ions (clay conductivity, Kc) and the contribution of the rest of the liquid (Kl). It should be realized that it is rather arbitrary to denote a certain part of the positive ions as counter ions and the rest of them as belonging to the interclay liquid. However, the second method is used mostly in the practice of conductance measurements of colloids. The major contributor to the conductance of the clay is the excess of ions at the interface of the clay water systems. By definition, the difference between the conductance in the range of the double layer and that in bulk solution is equal to the surface conductance. The ideal surface conductivity, K~, can be calculated by multiplying the ionic equivalent conductivity with the surface charge density. For Namontmorillonite this means
Ks =
LNa O
(1)
where Ks is the surface specific conductivity (mho), L~, is the Na equivalent conductivity (mho cm e equiv. 1), and a is the charge density at the clay surface (equiv. cm2). This calculation is based on the assumption that all sodium ions are distributed on an equipotential surface and their mobility is the same as that in a dilute aqueous solution. The definition is similar to the definition of the equivalent conductivity in salt solution, ~= Lc*, where L is the equivalent conductivity~ ~c is the specific conductivity, and c* is the concentration of the salt in equivalent per cm 3. The charge density of NaWyoming montmorillonite with a cation exchange capacity of 0"90mequiv.& and specific surface of 750m2/g, is 0.90 x 10 3 cr = 750 x 104 equiv'/cm2 = 1"18 x 101~ equiv./era 2 Thus, its ideal surface conductance at 25~ is K s : 50"1 x 118 x 101~ : 5'9 x 10~mho The two resistors in parallel model
The clay or the surface conductivity was defined as the difference between the conductance of the interface liquid and the conductance of the interclay solution. This is not an operational definition. In order to separate the experimental conductance of the gel, K,, into its componentsthe clay specific conductivity. K~, and the interclay specific conductivity, K~a model must be used. Meredith and Tobias (1962) reviewed and compared the equations developed for the calculation of the electrical conductivity of a mix
ture from the known conductivities of the separate phases, or vice versa, and found that rigorous solutions were available only for relatively simple cases (dilute suspensions, welldefined shape of the particles, no interaction, etc.). For more complicated systems, like clay gels, equations with empirical parameters should be introduced. The simplest and most widely used model considers the conductivity cell as consisting of two resistance elements in parallel (Fig. la). One component of the cell consists of the electrolyte in the interclay solution and another resulting from the contribution of the clay and the ions adsorbed on it. According to this model (van Olphen and Waxman, 1958; Cremers and Laudelout, 1966; Waxman and Smits, 1968), the electrical conductance of the gel, K9, is the sum of the surface and solution conductance, namely, K q = ~'c + ~q
(2)
where K9 is the specific conductivity of the gel, and Kc and ~ct are the conductances (not specific conductivity) of the clay and interclay solutions, respectively. Based on this model the surface conductivity of the clays may be calculated from the experimentally known electrical conductivities of the gel and the equilibrium solution. In equation (2), the specific conductivity of the gel is expressed in terms of the conductances of the cell components. In order to express the conductance of the components in terms of their specific conductivity, the geometry of the components and the tortuosity of the paths must be considered. This is usually done by introducing the formation factor, F (Cremers and Laudelout, 1965; Waxman and Smits, 1968), and the resulting equation is K9 = gc + KalE (3) where K9, Kc, and Kt are the specific conductivities of the gel, clay and liquid phase, respectively. The conductivity of the clay, Kc, can be determined by use of the isoconductivity point method (Dakshinamufti, 1960; Cremers and Laudelout, 1965). If the contribution of the clay conductance is constant, i.e. mobility of the exchangeable ions is constant, and I/F is not influenced by solution and clay concentration, then plotting gel conductivity, K o, vs solution conductivity, Kt, would form a straight line. From the slope of this line the formation factor is evaluated. The above assumptions do apply to the ELECTRODES ............
r
~
gp.rt!c{es~SOl~tio,
{' '
Model
I
ELECTRODES __~I
I : Resistors in parallel
Model 2 : Resistors in series
Fig. 1. Resistance models representing the clay particles and the interclay solution, d is the 'thickness' of the clay phase.
Electrical conductivity of Namontmorillonite suspensions electrical conductivity of clay gels at high electrolyte concentrations and equation (3) was used by Cremers and Laudelout (1966), Cremers et al. (1966) and Waxman and Smits (1968) to calculate the formation factors of their system. The tworesistorsinparallel model was applied in the following sections to analyze the experimental results.
207
ing way:
where k is a parameter which depends on the axial ratios of the solid particles. The values of k, as calculated from equation 4, are 26 and 24 for the 10 and 2"5 per cent clay, respectively. These values are intermediate between the values of k  13.9 obtained by EXPERIMENTAL PROCEDURE Cremers and Laudelout (1966), and the value of k = A clay size fraction of Upton Wyoming montmoril 52.9 obtained by Gast and Spalding (1966). (ii) The isoconductivity point. When the electrical lonite (API No. 25) was obtained by allowing large size fractions to settle out of suspension and then conductivity of a clay gel, Kg is compared to that siphoning off the suspension. Homoionic Naclay was of the solution, Kz, it is found that at low electrolyte prepared by saturating the colloid fraction with nor concentration, the conductivity of the gel is higher mal NaC1 solutions. This treatment was repeated four than that of the interclay solution. At high contimes. Thereafter, the clay was washed with distilled centrations of salt the opposite is true and the conwater in a highspeed centrifuge until tests with ductivity of the electrolyte solution is higher than that AgNO3 indicated that the equilibrium solution was of the gel. The relatively lower conductivity of the free of chloride. Then the clay was washed once more gel in the systems of high salt concentration is caused by interactions of electrolyte and water with the clay and the saltfree gel was freezedried and stored. The suspension was prepared by mixing known surfaces and the tortuosity of the paths. Conversely, weights of dry clay with equal volumes of NaC1 solu when the electrolyte concentration is low, the contritions of various initial concentrations. Seven con bution of the adsorbed ions and the clay macroions centrations of clay in the suspensions (0'1, 0"25, 0"5, to the conductivity of the gel is more effective than 1"0, 2"5, 6"0 and 8'0 per cent by weight) and three the reduction in the salt conductivity, so that Kg is NaC1 solutions (1 x 10 4, 1 x 103 and 3 x 103 N) higher than Kt. These relations are presented in Fig. were studied. In order to determine the isoconducti 3. The conductivity at which both effects balance each vity value and the formation factor of this clay, the other, namely when the gel conductivity is equal to electrical conductivities of two suspensions (1.0 and the conductivity of the interclay solution, is called 2'5 per cent by weight) in nine NaC1 solutions (0.0001, the isoconductivity point (Dakshinamurti, 1960; 0.001, 0.003, 0.01, 0"02, 0.04, 0'06, 0"08 and 0.1 N) were Cremers and Laudelout, 1965). As is evident from Fig. 3, the isoconductivity point of NaWyoming montexamined. The electrical conductivity of the solutions and of morillonite is 2.65 m mho/cm. This value agrees with the suspensions was determined with a Pyrex glass the values reported in the literature (Dakshinamurti, dip cell (Yellow Springs Instrument Co., YSI 3400) 1960; Cremers and Laudelout, 1965 and 1966). IG and a conductivity bridge (Industrial Instruments Inc., model RC 16 B2). The electrical conductivity e 2 . 5 % SUSPENSION / of suspensions that were equilibrated for 24 hr (at 25~ was measured. After the conductivity of the sus,o'~X"i/.o, pensions was measured, the suspensions were centri~ ~ ~ C Y '~ / /" fuged in a highspeed centrifuge, and the conductivity of the supernatant solution, K~, was determined.  , / o,~ / /
/
o.4L / /
RESULTS AND DISCUSSION
1. Effect of electrolyte concentration (i) The formation factor. The specific conductivity of 1.0 and 2.5 per cent Namontmorillonite suspensions as a function of the conductivity of NaC1 solutions is presented in Fig. 2. It is evident that in both suspensions there is an initial rapid increase in gell conductance which is greater than the conductivity of the added electrolyte alone. However, at the higher salt concentrations, a linear relation between the two axis is obtained with slopes of 0"885 and 081 for the 1'0 and 25 per cent clay, respectively. The corresponding F values (equation 3), are 113 and 1.235, respectively. Following Cremers and Laudelout (1966) and Cremers, Van Loon and Laudelout (1966), the formation factor is related to the porosity, qS, in the follow
0 '* C.
I
I
I
I
I
I
o
I
I
/
1 9% SUSPENSION
u_
I
0,4 I
I
o.a I
I
'o:, ' o ;I I I I
I
,
I
/
/
oO"~'~
o.s
i;i,/__
./
0.7
0.6 ~ U_ 0.5
~
3xI0"3N Ix I0"5N 04"~Iii~10"4N
~IKt..
z__ 0.4 9
WI~0.3 ~ t.L It. 0.2
3
3x103N N IxlO'3N
~ 0.1 I
I
I
1
I
I
2.0 4.0 6.0 CLAYCONCENTRATION (gm/lOOcc) Fig. 5. Differences between specific conductivities of suspensions Kg and original solutions, Ko, and between interclay solution, Kt, and original solutions, Ko, vs clay concentration, for three solution concentrations. sists of two resistance elements, the clay and the interclay solution, in series (Fig. Ib), while Gast used the model proposed by Spiegler et al. (1956), consisting of three components in parallel, one of which has its elements in series. Based on the two resistors in series model the specific resistance of the gel, in YL is the sum of the resistances of the elements, Rg = p c + p t
(6)
where Pc and p~ are the resistances of the clay and the interstitial liquid, respectively. The specific resistance of the clay, Re, a n d the liquid R~, are given by Ohm's law. P c = R f l and p ~ = R t ( 1  d ) (7) where d is the length parameter corresponding to the "thickness" of the clay phase (Fig. lb). The specific conductivity of the gel is given by
Kg
1
Rg

1
1
Pc + P~
Red + Rt(l  d)
KcKt = K t d + Kc(1  d)"
209
specific conductivity of the clay, Kc, as determined from the isoconductivity point. It is evident from Fig. 6 that, at the low range of salt concentration, the increase in the specific conductivity of the equilibrium solution results in a greater increase in the conductivity of the gel. This is in line with our experimental results (Figures 2, 4 and 5) and the results reported in the literature (Waxman and Smits, 1968). It is clear that this is a natural outcome of the model, which at the range of low salt concentration describes the claywater system more realistically, and it was not necessary to conclude that the mobility of adsorbed ions increases with an increase in the solution concentration. Comparing the experimental results (Figs. 2, 3 and 5) with the curves in Figure 6, one should note that the data of the 1"0 per cent suspension lies on the curve of d = 0"2, the data points of the 2'5 per cent clay lie on the curve ofd = 0"5 up to Kt  0'5 m mho; thereafter, the data points move in the direction of the d = 0'2 curve. Similarly, the data points of 6 per cent clay suspensions coincide with the d = 0'8 curve up to Kt = 0"5 m mho; thereafter, they deviate in the direction of the d = 05 curve. The volumetric fraction of the clay at the 10, 2'5 and 60 per cent by weight suspension is about 0.004, 0'01 and 0"024, respectively. Comparing the volumetric fraction of the clay particles with the volumetric fraction of the clay resistors in the model (d = 0.2, 0.5 and 0'8, respectively), it is evident that the "thickness" of the clay should include part of the diffuse double layer at each claywater interface. At the low range of salt concentration (